# data[].attributes.attachment_link.readable_text
Abstract

The cyclic deformation of VHB 4910 dielectric elastomer is experimentally investigated by performing a series of strain-controlled and stress-controlled pure-shear-like cyclic tests at room temperature. In the strain-controlled cyclic tests, obvious Mullins effect is observed in the first cycle, and continuous stress softening is characterized in the subsequent cycles; the Mullins effect and continuous stress softening are intensified by prescribing larger peak strains and higher strain rates. In the stress-controlled cyclic tests, remarkable ratchetting takes place, and its evolution becomes more significant if higher stress levels, lower stress rates and longer hold time at peak stress are prescribed. Moreover, a partial recovery of residual strain indicates that, besides obvious hyper-elasticity, the VHB 4910 dielectric elastomer also exhibits both recoverable viscoelasticity and measurable irrecoverable visco-plasticity during the cyclic tests.

Access options

Buy single article

Instant access to the full article PDF.

US$ 39.95

Tax calculation will be finalised during checkout.

Subscribe to journal

Immediate online access to all issues from 2019. Subscription will auto renew annually.

US$ 79

Tax calculation will be finalised during checkout.

References

1. 2.
Carpi F, De Rossi D, Kornbluh R, Pelrine RE, Sommer-Larsen P (2008) Dielectric elastomers as electromechanical transducers: fundamentals, materials, devices, models and applications of an emerging electroactive polymer technology. Elsevier

2. 4.
Gu G-Y, Zhu J, Zhu L-M, Zhu X (2017) A survey on dielectric elastomer actuators for soft robots. Bioinspiration & Biomimetics 12(1)

3. 7.
Kofod G (2001) Dielectric elastomer actuators: Ph. D. Thesis. The Technical University of Denmark

4. 21.
Chen K, Kang G, Lu F, Jiang H (2015) Uniaxial cyclic deformation and internal heat production of ultra-high molecular weight polyethylene. J Polym Res 22(11)

5. 26.
Vertechy R, Fontana M, Stiubianu G, Cazacu M (2014) Open-access dielectric elastomer material database. In electroactive polymer actuators and devices. Proc of SPIE, San Diego, California. https://doi.org/10.1117/12.2045053

6. 27.
Zhou J, Jiang L, Khayat RE (2018) A micro-macro constitutive model for finite-deformation viscoelasticity of elastomers with nonlinear viscosity. Journal of the Mechanics and Physics of Solids 110:137-154. https://doi.org/10.1016/j.jmps.2017.09.016

Download references

Acknowledgements

This work is financially supported by National Natural Science Foundation of China (11272269 and 11572265), the Opening Project of Applied Mechanics and Structure Safety Key Laboratory of Sichuan Province, China (SZDLH-1702) and Doctoral Innovation Fund Program of Southwest Jiaotong University (D-CX201837).

Author information

Affiliations

1. State Key Laboratory of Traction Power, Southwest Jiaotong University, Chengdu, 610031, Sichuan, China

Yifu Chen & Guozheng Kang

2. Applied Mechanics and Structure Safety Key Laboratory of Sichuan Province, School of Mechanics and Engineering, Southwest Jiaotong University, Chengdu, 610031, Sichuan, China

Yifu Chen, Guozheng Kang & Jianghong Yuan

3. Department of Engineering Mechanics, Zhejiang University, Zhejiang, 310027, Hangzhou, China

Tiefeng Li

Corresponding author

Correspondence to Guozheng Kang.

Additional information

Publisher's note

Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.

About this article

Cite this article

Chen, Y., Kang, G., Yuan, J. et al. Experimental study on pure-shear-like cyclic deformation of VHB 4910 dielectric elastomer. J Polym Res 26, 186 (2019). https://doi.org/10.1007/s10965-019-1858-6
Download citation
Keywords

Dielectric elastomer

Cyclic deformation

Time-dependence

Stress softening

Ratchetting

# data[].attributes.attachment_link.title
Experimental study on pure-shear-like cyclic deformation of VHB 4910 dielectric elastomer

# data[].attributes.attachment_link.description
The cyclic deformation of VHB 4910 dielectric elastomer is experimentally investigated by performing a series of strain-controlled and stress-controlled pure-shear-like cyclic tests at room temperature. In the strain-controlled cyclic tests, obvious Mullins effect is observed in the first cycle, and continuous stress softening is characterized in the subsequent cycles; the Mullins effect and continuous stress softening are intensified by prescribing larger peak strains and higher strain rates.

# data[].attributes.body
doi:10.1002/app.42135

# data[].attributes.body
https://youtu.be/nNn4Lpd4uBM

# data[].attributes.body
https://doi.org/10.1016/j.vibspec.2019.102994

# data[].attributes.body
Forma de aplicarlo podría influir en la "actuación" del material/elastómero.
Campo eléctrico más heterogeneo si las láminas están distribuidas heterogeneamente.
Grosor debe ser controlado, control en campo eléctrico.
Uniformidad del campo eléctrico es importante.
Sumas vectoriales en estado "micro"

# data[].attributes.body
en el video 2 el tipo hace una exfoliación mecánica con el maso de un mortero, los otros 2 deberían emularlo

# data[].attributes.body
Polímeros podrá considerarse electroactivo si este preseta en su estructura molecular grupos polares, si tb presenta estructuras entrecruzadas, que cuelgan de una cadena principal
Crosslinker polar, cambia polaridad y orientación al estirarlo. Reordenamiento
O, S destacan como átomos polarizables cuando están dentro de cadenas poliméricas.
Capa conductora debe aplicarse homogeneamente para que campo eléctrico sea homogéneo.

# data[].attributes.body
al estirar el film el grosor final debe ser controlado

# data[].attributes.body
cuando se agrega el carbonaceo, se debe usar una tecnica que deje las estructuras mas homogenas, como un coating por inmersion o spray

# data[].attributes.body
DOI: 10.1002/anie.201301918

# data[].attributes.body
https://link.springer.com/article/10.1007/s10965-019-1858-6

# data[].attributes.body
https://doi.org/10.1016/j.polymer.2018.06.065

# data[].attributes.attachment_link.readable_text
Introduction

Dielectric elastomers (DEs) are a class of smart materials that have the ability to convert mechanical energy into electrical energy and vice versa. The basic structure of a dielectric elastomer actuator (DEA) device is composed of a DE film sandwiched between two compliant conductive electrodes. When a DEA is subjected to a voltage, opposite charges accumulate at the two electrodes, leading to compression of the DE film due to the Maxwell pressure P. As a result of this compressive force, the thickness of the DE film is reduced while the area expands. The Maxwell pressure P generated is expressed in Eq. 1, where ε ₀ is the vacuum permittivity, ε is the dielectric constant, V is the voltage applied across the dielectric and z is the thickness of the dielectric material. At strains <20%, the DE response is often assumed to be linear, and the actuation strain incurred by the DE in the thickness direction is estimated through Eq. 2, where Y is the elastic modulus and S z is the strain in the thickness direction.

$$P = \varepsilon _0\varepsilon \left( {\frac{V}{z}} \right)^2$$

$$S_Z = \frac{1}{Y}\varepsilon _0\varepsilon \left( {\frac{V}{z}} \right)^2$$

Currently, commercially available acrylate-based (e.g., VHB TM) polymers are often used for DEAs because they exhibit large area strains up to 380% and possess relatively high dielectric constants (≈4.7) and breakdown field strengths. However, commercial VHB polymers exhibit slow response and recovery times of several hundred seconds due to their highly viscoelastic nature. In addition, as a dissipative process, viscoelastic hysteresis has been shown to exert an adverse effect on performance and cause positioning inaccuracy. To circumvent these issues, materials with low viscoelasticity, such as silicone rubber, are often used to replace VHB polymers. However, these nonpolar polymers exhibit a low dielectric constant (≈2.8), which is a critical parameter to achieve high strains in DEAs, as observed from Eq. 1. Hence, a large number of studies have focused on increasing the dielectric constant for improved actuation performance of DEAs, thereby achieving a higher area strain and work density. The general approaches that have often been investigated include the addition of ceramic particles with high dielectric permittivity, the addition of conductive nanofillers and chemical modification to introduce polar groups. Alternatively, DEAs have been prestretched to reduce the effects of viscoelasticity. Some studies have shown that prestretching provides benefits such as a shorter relaxation time, reduced drifting effects and higher electromechanical strain. However, the prestretched state is often achieved by mounting the DE film on a rigid frame, which increases the weight of the actuator and limits the incorporation of DEAs into soft and flexible bodies. Additionally, prestretching reduces the lifetime of the device due to stress relaxation and fatigue.

In this work, we designed and prepared a copolymerized polyurethane acrylate (PUA)-based DEA that avoids prestretching and realizes fast response and stable recovery. This goal is achieved by introducing chemical crosslinks to tune the viscoelasticity caused by the sliding of polymer chains across each other. Although the presence of these chemical crosslinks increases the elastic modulus of the DE, the introduction of polar groups that are present in the comonomer enhances the dielectric constant of the DE, counteracting its impact on actuation performances such as the maximum area strain and work density. We present a buckling-mode DEA, which exhibits out-of-plane deflection without prestretching, based on a copolymer with tunable properties provided by adjusting the crosslinking density. At higher crosslink densities, minimal actuation drifts upon cycling can be realized, and response times of <1 s have been achieved, which is a substantial feat for DEAs. The rapid response and stable cycling of DEAs make them attractive for integration into soft bodies or wearable textiles, expanding the capabilities of DEAs for tactile sensing, haptic feedback, and soft robotics.

Materials and methods

Materials

CN9021, an aliphatic urethane acrylate oligomer developed for laminating and pressure sensitive adhesives, was purchased from Sartomer Company and was used as received. Polyethylene glycol diacrylate (PEGDA) with a molecular weight of 575 and azobisisobutyronitrile (AIBN) was obtained from Sigma Aldrich and was used as received. Carbon grease was purchased from Nanjing Xilite Adhesive Co. Ltd and was used as received.

Synthesis of PUA-PEGDA copolymer films

CN9021 was mixed with different concentrations of PEGDA (5, 10, and 15 wt%), and 1 wt% of AIBN was added to the mixture and mixed thoroughly. The resultant precursor solution was then cured on a hotplate in an inert environment at 90 °C for 1 h. Polymer films were carefully peeled out, and an average film thickness of 0.43 mm was obtained. Pristine CN9021 films were denoted as PUA, whereas copolymer films were denoted as PUA-PEGDA-X, with X representing the weight percent of PEGDA.

Characterization of chemical structure

Fourier transform infrared (FTIR-ATR, Perkin Elmer, Frontier) spectroscopy was used to measure the FTIR spectra by scanning each film 32 times with a resolution of 4 cm −1.

Characterization of dielectric properties

Dielectric constant measurements were performed in the frequency range of 1 kHz to 1 MHz using an Agilent E4980a LCR meter. An AC signal of 1 V was applied to the samples, and the dielectric constant was calculated from the capacitance measured with the following relationship: C = ( ε ₀ ε Α)/ d, where A is defined as the overlapping area between the top and bottom electrodes, ε ₀ is the vacuum permittivity, C is the measured capacitance, and d is the polymer film thickness. Elastomer samples were placed between two electrodes for measurements.

Characterization of mechanical properties

Tensile test specimens were prepared in accordance with ASTM D638-14, Type V. Tensile tests were performed on an Instron 5567 universal testing machine at a strain rate of 3.33 mm s −1. Loading and unloading cyclic tests were performed at a strain rate of 1.0 mm s −1 for 30 cycles with a limiting strain of 100%.

Actuator fabrication

Polymer films with an average thickness of 0.43 mm were placed on an in-house glass holder prepared with a 2 cm × 2 cm hole to allow out-of-plane actuation. Carbon grease was used as the electrode, which was coated over a circular area with a diameter of 3 mm on the top and bottom surface of the film. Copper tape was used to provide electrical connection to a Unicorn UHP-75 high voltage DC power supply.

Characterization of actuation performance

The vertical deflection from the center of the electrode was determined with an Epsilon optoNCDT laser displacement sensor. For static actuation experiments, the voltage was increased by 0.5 kV every 10 s. Actuation strains were determined by calculating the change in the electrode area through geometric relations. Cyclic actuation measurements were performed using a Trek TM Model PD05034 high voltage AC power amplifier to amplify the signal generated from the pulse generator. The cyclic measurements were performed at a frequency of 0.5 Hz with an electric field strength of 10 V μm −1. To evaluate the response times, the generated wave profiles were obtained at a frequency of 0.1 Hz with an electric field strength of 10 V μm −1. The response time t 0.9 of the actuator was quantified by the time taken to reach 90% of the maximum displacement for each cycle. Three samples were tested for each copolymer formulation.

Results and discussion

PUA-PEGDA structure

PUA, consisting of a flexible polyether diol segment and a relatively flexible di-isocyanate segment, was copolymerized with PEGDA (Fig. 1a-c) of low molecular weight (Mw = 575). To verify the successful copolymerization between the two compounds, FTIR (Fig. 1e) and NMR (Figs. S 1- 3, Supplementary Information) measurements were performed. FTIR measurements of the pristine PUA displayed absorption peaks for CH ₂ at 2940 cm −1 (-CH stretching consisting of asymmetric -CH ₃ stretching at 2955 cm −1, asymmetric -CH ₂ stretching at 2924 cm −1, symmetric -CH ₃ stretching at 2873 cm −1 and symmetric -CH ₂ stretching at 2857 cm −1), H-C-H scissor bending at 1457 cm −1 and =CH stretching at 810 cm −1. For PUA-PEGDA copolymers, the appearance of strong characteristic peaks (Table S1, Supplementary Information), such as the stretching vibrations of −NH− at 3350-3200 cm −1, C=O at 1720-1727 cm −1, C=C at 1635 cm −1 and -NH- at 1520-1580 cm −1, confirms the formation of crosslinks between PEGDA and PUA through free radical polymerization. Furthermore, the spectra do not show the characteristic peak of -NCO at 2260-2270 cm −1, indicating a complete usage of the isocyanate upon copolymerization. With the successful copolymerization of the two components, a chemical crosslink network between polymer chains is established, preventing the chains from slipping across one another (Fig. 1d).

Chemical structures of a PUA, b PEGDA, and c PUA-PEGDA copolymer. d Schematic illustration of crosslinking network structures with PUA-PEGDA. e FTIR spectra of PUA and PUA-PEGDA copolymer films (5, 10, and 15 wt%) measured over the range of 400-4000 cm −1

Dielectric properties of the PUA-PEGDA copolymer

The dielectric permittivity of the copolymer films with various concentrations of PEGDA is shown in Fig. 2a. With an increase in PEGDA concentration, a drastic improvement in the permittivity is observed. The dielectric permittivity increases from 5.52 to 8.87 at 1 kHz (Fig. 2b), whereas the commercial VHB 4905 (for comparison) has a measured permittivity of 4.4 at 1 kHz. This improvement can be attributed to the increase in polarity of the copolymer film due to the increasing number of C-O bonds introduced into the polymer with increasing PEGDA content. This finding indicates that the dielectric properties of the films can be tuned by controlling the concentration of PEGDA. This realization is critical because the dielectric permittivity is proportional to the generated Maxwell pressure. As the frequency increases, the permittivity of the copolymer decreases, as illustrated in Fig. 2a. This phenomenon is typically related to dielectric relaxation, in which the polar groups on the polymer chains are unable to keep up with the alternating current, resulting in a loss of contribution to the dielectric permittivity.

a Dielectric constants of PUA, PUA-PEGDA copolymer films (5, 10, and 15 wt%) and VHB 4905 measured over a frequency range of 1 kHz to 1 MHz. b Dielectric constants of copolymer films at various PEGDA concentrations measured at 1 kHz. Three samples were measured for each concentration

Mechanical properties of the PUA-PEGDA copolymer

The effects of chemical crosslinks between PEGDA and pristine PUA on the mechanical properties can be observed from the stress-strain curves in Fig. 3a. Copolymer films with concentrations up to 10 wt% of PEGDA exhibited a nonlinear behavior with a slow, gradual increase in stress at low strains due to the unfolding of polymer chains. However, at larger strains, the elastomer exhibits a strain hardening behavior with a rapid increase in the elastic modulus as the polymer chains begin to become taut and aligned. This elastomeric behavior is a characteristic of many other elastomers, such as polyurethane and VHB polymers. At 15 wt% of PEGDA, the nonlinear elastomeric behavior was attenuated accompanied by a reduced maximum attainable elongation due to an increase in crosslinking. This phenomenon was accompanied by a reduction in the apparent modulus, which may be attributed to an increase in length between crosslink junctions as the probability of PEGDA acrylate groups reacting with each other increases at higher concentrations. As the number of chemical crosslinks between PEGDA and PUA polymer chains increases, the mobility of the chains is severely restricted, reducing the maximum elongation to 167% from the 960% elongation of the pristine PUA. Note that the maximum elongation at 15 wt% of PEGDA is comparable to the maximum elongation of polydimethylsiloxane (PDMS) (Sylgard 184) by Dow Corning. A summary of the mechanical properties of the fabricated films is provided in Table 1.

a Stress-strain curves of PUA and PUA-PEGDA copolymer films (5, 10, and 15 wt%) determined from a standard tensile test at a displacement rate of 3.33 mm s −1. The inset image shows magnification at low tensile strains between 0 and 200%. Loading and unloading cyclic tests performed on b PUA, c PUA-PEGDA-5, d PUA-PEGDA-10, and e PUA-PEGDA-15 at a strain rate of 1 mm s −1 for 30 cycles, showing the reduction in hysteresis loss

Table 1 Mechanical properties of PUA and PUA-PEGDA copolymers

To evaluate the viscoelastic behavior of the fabricated copolymers, loading-unloading cyclic tests were performed for 30 cycles at a strain rate of 1 mm s −1. From the experiments (Fig. 3b-e), all samples exhibited hysteresis loss, which is represented by the area enclosed in the curve. This area represents the energy dissipated during cycling, which is related to the internal friction and sliding of polymer chains in viscoelastic elastomers. As a result of the Mullins effect, a large hysteresis loss during the first cycle was observed for all samples, wherein the largest loss was displayed by the pristine PUA sample. After the second cycle, the stress-softening behavior during cyclic loading begins to reach a stationary state with a stable hysteresis loop being formed. A reduction in hysteresis loss after the first cycle can be observed with increasing PEGDA concentration, which occurs because the increasing crosslinking density between polymer chains restricts motion and lowers the dissipative energy. Moreover, the reduction in hysteresis implies a reduced viscoelastic loss, which can be correlated to improved electromechanical stability through cycling tests of up to 1050 cycles (Figs. S7- 10, Supplementary Information); this phenomenon aided in the enhanced dynamic response times of the actuator, which will be elaborated later.

Static performance of buckling-mode DEA

To demonstrate an entirely flexible device, a buckling-mode actuator was set up under prestretch-free conditions. Carbon grease was coated on both surfaces with a circular overlapping region, which is defined as the electroactive region. Buckling of the film occurs as the electroactive region expands against the passive region of the DEA with no overlapping electrodes. This phenomenon creates a boundary condition that suppresses the lateral expansion of the electroactive region and generates a compressive stress across the DE. When the buckling limit is exceeded, out-of-plane deflection is achieved as the film buckles. The actuated out-of-plane displacement was measured using a laser displacement sensor (Fig. 4a, b). Area strains were determined from changes in the electroactive areas through geometric relations, whereas deflection strains (Fig. S5) were based on deflection-to-thickness ratios. Figure 4c and Fig. S6 show that the pristine PUA exhibits a sudden increase in area strain before dielectric breakdown, which was not observed in the PUA-PEGDA copolymers (PUA-PEGDA-X, where X is the wt% of the PEGDA). This finding is attributed to the nonlinear behavior of PUA, for which the modulus becomes significantly smaller than that of the PUA-PEDGA copolymers (Fig. 3a) beyond 10% strain. The early breakdown of PUA is expected without the application of prestrains to prevent electromechanical instabilities. In contrast, copolymers with higher concentrations of PEGDA (10 wt% and 15 wt%) could be tested beyond the breakdown strength of pristine PUA and PUA-PEGDA-5 because the increase in stiffness from chemical crosslinks lowers the likelihood of electromechanical instabilities. With this effect, PUA-PEGDA-10 and PUA-PEGDA-15 could be tested at higher electric field strengths to achieve higher maximum strains than PUA or PUA-PEGDA-5. A comparison between the area strains of the DEA materials with no prestrains is presented in Table 2. In comparison to low viscoelastic materials, such as silicone, PUA-PEGDA-15 displayed higher area strains under lower electric field strengths without prestretching. This finding can be attributed to the high dielectric permittivity, which led to a higher generated Maxwell pressure.

Actuation of a single buckling-mode dielectric elastomer actuator (DEA) in the a off state and b on state, where Δ h represents the displacement achieved when a voltage is applied. c Representative area strains of PUA and PUA-PEGDA copolymers (5, 10, and 15 wt%) with increasing electric field strength. d Estimated work density based on measured area strains of PUA and PUA-PEGDA copolymers (5, 10, and 15 wt%) with increasing electric field strength

Table 2 Comparison of area strain between DEA materials without prestrains

Under an isochoric assumption, the work density ( u e) of the material was calculated as the work done by the actuator divided by its volume, as shown in Eq. 3, where P represents the generated Maxwell pressure and s z is the thickness strain determined from the measured area strains.

As shown in Fig. 4d, the reduction in the work density that arose from the increased crosslinking with increasing PEGDA concentration was gradually minimized. At electric field strengths of up to 15 V/μm, the work density of PUA-PEGDA-15 was similar to that of the pristine PUA sample, indicating an optimum balance between the effects of the increased dielectric constant and the elastic modulus. Furthermore, as PUA-PEGDA-15 could be tested at higher electric field strengths, the maximum work density achieved by PUA-PEGDA-15 was the highest among the measured samples; this evidently shows the effectiveness of polar crosslinks for increasing the load that the actuators are capable of driving.

Dynamic performance of a buckling-mode DEA

The dynamic performance and endurance of the buckling-mode actuator were evaluated through cyclic tests performed at a frequency of 0.5 Hz for 1050 cycles (Movie S1, Supplementary Information). To evaluate the effects of the viscoelastic drift, we presented the first 145 cycles (Fig. 5a-d); subsequent cycles are presented in Figs. S6- 9 in the Supporting Information. Samples of PUA and PUA-PEGDA-5 were observed to gradually drift from their equilibrium position by a large amount (>0.15 mm) before reaching a stable state. Such behavior is the result of the inherent viscoelastic characteristics of the film, wherein the relaxation time is slower than the cycling time, and the energy is dissipated from the sliding of the polymer chains across each other. Similar behaviors have been observed in elastomers with high viscoelasticity, such as VHB polymers. The introduction of PEGDA as chemical crosslinks, which anchor the polymer chains to reduce molecular motion, results in better thermal stability (Fig. S4), faster relaxation time and minimal drift of the DEA. These findings are evident from Fig. 5d, as the viscoelastic drift decreases significantly for the PUA-PEGDA-15 samples. At the end of 145 cycles, PUA drifted a distance of 0.28 mm from its initial start point, whereas PUA-PEGDA-15 drifted a distance of only 0.09 mm. With reduced viscoelastic drift, better location precision can be obtained. In addition, by tuning the viscoelastic nature of the polymer films, the response times of the actuator can be controlled. To allow sufficient time for the peak displacement to be reached, the voltage was applied at 0.1 Hz. The response time t 0.9 of the actuator was quantified as the time taken to reach 90% of the maximum displacement for each cycle. From Fig. 5f, PUA-PEGDA-15 achieved a response time of <1 s, which is an improvement compared to PUA; this finding was corroborated by the reduced hysteresis loss tested earlier. The strain response (Fig. 5e) of the synthesized PUA-PEGDA-15 is analogous to that of silicones with higher elastic properties, lower dissipative energy and a faster response time.

First, 145 cycles of the cyclic test were performed at an electric field strength of 10 V μm −1 at a frequency of 0.5 Hz for a PUA, b PUA-PEGDA-5, c PUA-PEGDA-10, and d PUA-PEGDA-15. The approximate drift distance after 145 cycles is stated in red. Profile of a single cycle of e the strain response of PUA and PUA-PEGDA-15 under a 10 V μm −1 electric field at 0.1 Hz is shown to demonstrate the difference in response time, t 0.9. This response time t 0.9 represents the time for the actuator to reach 90% of its maximum displacement at 0.1 Hz. f Response time t 0.9 at various PEGDA concentrations (0, 5, 10, and 15 wt%)

To demonstrate the provision of pixelated actuation, we extended the localized actuator into an array through a cross-junction design configuration where three actuators can be activated simultaneously (Fig. 6a). The fabricated actuator array with a cross-junction configuration can be realized on a flexible substrate without a rigid frame or prestretching, as shown in Fig. 6b and Movie S2 in the Supporting Information. The conceptualization of the fabricated actuator array integrated into a watch strap to provide haptic feedback for wearables can be found in Fig. 6c and Movie S3.

a Schematic of an actuator array in a cross-junction configuration. Electrical connections are connected to activate the middle three actuators. b Fabricated actuator array in a cross-junction configuration on a flexible substrate. c Conceptualization of the fabricated actuator array integrated into a watch strap to provide haptic feedback for wearables

Conclusion

In this work, we presented an approach to tune the viscoelastic properties of a DEA for improved dynamic performance. Through the addition of low molecular weight PEGDA, we increased the number of chemical crosslinks within the polymer matrix, thereby anchoring the polymer chains. As a result, the slipping of the polymer chains across each other is minimized, thereby reducing the viscoelastic effects. This phenomenon is supported by the reduction in hysteresis loss during mechanical cyclic loading with increasing PEGDA concentrations as energy dissipation from molecular motion is reduced. To verify our hypothesis, we fabricated a buckling-mode actuator and performed cycling experiments. The response times were reduced by more than 50% with increasing PEGDA concentrations, reaching 90% of the maximum amplitude in <1 s. In addition, stable and reliable performance was observed with a significant reduction in viscoelastic drifts with increasing PEGDA concentration, allowing the potential usage of the proposed DEA for high precision applications, such as tunable lenses and gratings. Although the increase in the number of crosslinks was shown to increase the elastic modulus of the material, by introducing polar groups present in PEGDA, we were able to achieve a maximum area strain that was notably higher than low viscoelastic materials, such as silicone, which requires a larger operating voltage. Furthermore, our device avoids the use of rigid components used to achieve a prestretched state for reduced viscoelastic effects and improved actuation performances. This capability allows the fabricated copolymer to be integrated into soft and flexible bodies, highlighting a promising approach for faster, stable, and flexible actuators.

Acknowledgements

This research was financially supported by the Competitive Research Programme Award no. NRF-CRP-13-2014-02 and the NRF-Investigatorship Award no. NRF-NRFI2016-05 provided by the National Research Foundation, Singapore. M.W.M.T acknowledges the scholarship awarded by the Nanyang Technological University, Singapore.

Author information

Affiliations

School of Materials Science and Engineering, Nanyang Technological University, 50 Nanyang Avenue, Singapore, 639798, Singapore

Matthew Wei Ming Tan, Gurunathan Thangavel & Pooi See Lee

Corresponding author

Correspondence to Pooi See Lee.

Ethics declarations

Conflict of interest

The authors declare that they have no conflict of interest.

Additional information

Publisher's note Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.

Supplementary information

Rights and permissions

Open Access This article is licensed under a Creative Commons Attribution 4.0 International License, which permits use, sharing, adaptation, distribution and reproduction in any medium or format, as long as you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made. The images or other third party material in this article are included in the article's Creative Commons license, unless indicated otherwise in a credit line to the material. If material is not included in the article's Creative Commons license and your intended use is not permitted by statutory regulation or exceeds the permitted use, you will need to obtain permission directly from the copyright holder. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/.
Reprints and Permissions

About this article

Cite this article

Tan, M.W.M., Thangavel, G. & Lee, P.S. Enhancing dynamic actuation performance of dielectric elastomer actuators by tuning viscoelastic effects with polar crosslinking. NPG Asia Mater 11, 62 (2019). https://doi.org/10.1038/s41427-019-0147-5
Download citation

Further reading

Ardi Wiranata

& Shingo Maeda

Key Engineering Materials (2021)

Ardi Wiranata

, Yasuyuki Ishii

, Naoki Hosoya

& Shingo Maeda

Advanced Engineering Materials (2021)

Junshi Zhang

, Liling Tang

, Lei Liu

, Jianwen Zhao

, Zhichun Yang

& Pengfei Li

International Journal of Mechanical Sciences (2021)

Dinorath Olvera

& Michael G. Monaghan

Advanced Drug Delivery Reviews (2021)

Mengmeng Han

, Ling Liu

, Jinming Yuan

& Liqun Zhang

Polymer Composites (2021)

# data[].attributes.attachment_link.title
Enhancing dynamic actuation performance of dielectric elastomer actuators by tuning viscoelastic effects with polar crosslinking

# data[].attributes.attachment_link.description
Dielectric elastomer actuators (DEAs) often suffer from time-dependent deformations due to their inherent viscoelastic properties. Herein, the viscoelastic effects were tuned through copolymerization between a polar crosslinker and a polyurethane acrylate DEA. With polar groups present in the crosslinker, the dielectric constant was effectively increased, achieving higher area strains compared to that exhibited by low viscoelastic elastomers such as silicone.

# data[].attributes.body
10.1002/mame.201400122

# data[].attributes.body
10.1002/mame.201400122

# data[].attributes.body
C 1rios y 2rios
CH2
Carbonilo
Cadenas con átomos electronegativos y formando enlaces polares (O, S)

# data[].attributes.body
Aporte desde el laboratorio ¿Críticas a la forma de ejecutar?
- Uso de guantes y EPP: carbon (grafeno, grafito, CNTs.etc)
- Pasta de plata

# data[].attributes.body
Dielectric polymers are able to hold their induced displacement while activated under a DC voltage. This allows dielectric polymers to be considered for robotic applications. These types of materials also have high mechanical energy density and can be operated in air without a major decrease in performance. However, dielectric polymers require very high activation fields (>10 V/µm) that are close to the breakdown level.

The activation of ionic polymers, on the other hand, requires only 1-2 volts. They however need to maintain wetness, though some polymers have been developed as self-contained encapsulated activators which allows their use in dry environments. Ionic polymers also have a low electromechanical coupling. They are however ideal for bio-mimetic devices.

# data[].attributes.body
VHB 4910 ¿estructura molecular?
https://www.researchgate.net/publication/271933456_Thermal_Mechanical_and_Dielectric_Properties_of_a_Dielectric_Elastomer_for_Actuator_Applications
https://makezine.com/2012/01/26/shapeshift-electroactive-polymer-sheets/
https://www.youtube.com/watch?v=PgNKeqOCOKE
https://www.youtube.com/watch?v=aBAzjJwFkS0
https://www.youtube.com/watch?v=eUdcBjo19oU

# data[].attributes.body
con capacidad de cambiar de forma y tamaño al aplicarle/exponerlo a un campo eléctrico externo